Advances in Condensed Matter Physics
Volume 2019 (2019), Article ID 6179456, 5 pages
https://doi.org/10.1155/2019/6179456

Research Article

Physical Structure Induced Hydrophobicity Analyzed from Electrospinning and Coating Polyvinyl Butyral Films

Shuo Chen,¹ Guo-Sai Liu,¹ Hong-Wei He,¹ Cheng-Feng Zhou,² Xu Yan,1,3,4 and Jun-Cheng Zhang⁴

¹Industrial Research Institute of Nonwovens and Technical Textiles, College of Textiles and Clothing, Qingdao University, Qingdao 266071, China
²State Key Laboratory of Bio-Fibers and Eco-Textiles, Qingdao University, Qingdao 266071, China
³Collaborative Innovation Center for Eco-Textiles of Shandong Province, Qingdao University, Qingdao 266071, China
⁴Collaborative Innovation Center for Nanomaterials and Optoelectronic Devices, College of Physics, Qingdao University, Qingdao 266071, China

Correspondence should be addressed to Cheng-Feng Zhou; chengfengzhou@qdu.edu.cn and Xu Yan; yanxu-925@163.com

Received 5 November 2018; Accepted 5 March 2019; Published 1 April 2019

Academic Editor: Golam M. Bhuiyan

Copyright © 2019 Shuo Chen et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Surface wettability of a film plays a critical role in its practical applications. To control the surface wettability, modification on the physical surface structures has been a useful method. In this paper, we reported the controlling physical surface structure of polyvinyl butyral (PVB) films by different film-forming methods, spin-coating, bar-coating, and electrospinning. The wettability of these PVB films was examined, and the surface morphologies and roughness were investigated. The results indicated that coating PVB films were hydrophilic, while electrospun films were hydrophobic. The physical surface structure was the key role on the interesting transition of their surface wettability. Theoretical analyses on these results found that the coating PVB films showed different mechanism with electrospun ones. These results may help to find the way to control the PVB film surface wettability and then guide for applications.

1. Introduction

The wetting behavior of solid surfaces by a liquid as a very important aspect of surface properties has been a focused interest for a long time [1–4] and has shown a wide variety of practical applications in various fields, such as protecting clothes [5], medical care [6–8], and filtration [9]. Consequently, great efforts have been made to find the way to control the surface wettability [10–13].

According to the term biomimetic, “lotus leaves effect” indicates that the cooperation of hierarchical structures and other specific components on the natural surfaces results in the desired wettability [1–3, 14]. Moreover, from the theoretical view, such as Young’s equation [15], Wenzel model [16], and Cassie model [17], the surface roughness plays a critical role in surface wettability [18–21]. Furthermore, the rough surface is extended to porous surfaces and even micro-nano structures [22–24]. To achieve these structures, especially in film structures, several methods are developed such as solution cast and electrospinning [5–10, 19, 21].

Among various materials, polyvinyl butyral (PVB), which is characterized by high adhesion to glass, excellent mechanical strength, excellent biocompatibility, nontoxicity, and good solubility in alcohol, has been applied to many fields such as an adhesive interlayer in safety glass, wound dressing, and coating film [5–7, 10, 11]. Moreover, PVB shows both hydrophobic and hydrophilic properties due to its chemical structure with both vinyl butyral group and vinyl hydroxyl group [10, 25]. And previous study has suggested that electrospun PVB nanofibrous structures and patterns showed larger water contact angle (WCA) than that of the solution casting film [7, 10, 11]. However, these works most focus on the electrospun PVB meshes and rarely discuss the comparison of the structures between the different methods.

In this paper, we focused on the comparison of PVB films made by several methods, spin-coating, bar-coating, and electrospinning. The WCAs on these films were measured and the morphologies and surface roughness of them were also examined. By analyzing these results, we want to find a way to control the surface wettability.

2. Materials and Methods

2.1. Materials

Polyvinyl butyral (PVB) (MW~100,000, Sinopharm Chemical Reagent Co., Ltd., China) was dissolved in ethyl alcohol (analytical reagent, 99%) at 8 wt%, 10 wt%, and 12 wt% firstly and then stirred for 2 h at room temperature.

2.2. Preparation of the Films

The PVB/alcohol solutions were used to produce films by spin-coating, bar-coating, and electrospinning, respectively. During spin-coating process, PVB/alcohol solutions were dripped onto cover slips (20 mm×20 mm) with 5 μl and then set on the spin-coater (KW-4A, Institute of Microelectronics of the Chinese Academy of Sciences). The spinning velocities were selected at 250 r/s, 300 r/s, and 350 r/s, and spinning time was set at 30 seconds. In bar-coating process, 10 μl PVB/alcohol solutions were dripped onto slide glasses (76 mm×26 mm), and the bars were selected with 6 μm, 8 μm, and 10 μm film thickness. For electrospun meshes, both positive electrospinning and negative electrospinning were processed. PVB/alcohol solutions were firstly loaded into syringes (5 ml) and then set on the electrospinning apparatus (DW-P303-1ACF5 (positive), DW-N303-1ACDF0 (negative), Dongwen, China), the electrospinning voltage was set at 15 kV and -15 kV, and the distances were selected at 15 cm, 20 cm, and 25 cm.

2.3. Characterization

The static water contact angles (SWCA) of the prepared films were examined by an optical tensiometer (Attension Theta, Biolin Scientific, Germany) with a 2 μL water droplet for three sites at room temperature and analysis was performed by fitting drops with a Young-Laplace formula using the Theta software. The surface roughness was also measured by optical tensiometer with 3D surface roughness module. The morphologies of the films were examined by a scanning electron microscope (SEM, Phenom ProX, Phenom Scientific Instruments Co., Ltd., China) at 10 kV, and all samples were coated with gold for 30 s before analysis. The fiber diameters were analyzed by Nano Measurer software. The Fourier transform infrared spectroscopy (FTIR) spectrums were measured by a Thermo Scientific Nicolet iN10 spectrometer.

3. Results and Discussion

To ensure the wettability of the prepared PVB films, SWCA were measured and shown in Table 1. One can find that the spin-coating and bar-coating PVB films showed hydrophilicity with SWCA <90°, while the electrospun films showed hydrophobicity with SWCA>90°, which agreed with the previous study [7, 10, 11]. Moreover, the bar-coating PVB films had larger SWCA than spin-coating ones generally. The SWCA of electrospun PVB films with positive electrospinning process is mostly larger than that of negative electrospinning. Nevertheless, as seen from Figure 1, the prepared PVB films showed similar absorption peaks, which indicated that these films had same chemical structures. It is interesting that the same material showed different wettability for its different film-forming methods.

Table 1: The SWCA of the prepared PVB films by different methods.

Methods
SWCA (°)
SWCA (°)
SWCA (°)
ASWCA (°)

Concentrations/parameters
8 wt%
10 wt%
12 wt%

Spin-coating
250 r/s
77.767
78.800
78.900
78.593

300 r/s
74.300
82.600
79.933

350 r/s
76.033
82.733
76.267

Bar-coating
6 μm
86.438
83.297
84.303
83.067

8 μm
81.255
82.626
81.437

10 μm
81.093
81.360
85.796

Positive electrospinning
15 cm
135.833
130.833
131.933
132.404

20 cm
132.167
133.600
129.700

25 cm
131.667
135.400
130.500

Negative electrospinning
15 cm
131.033
135.733
130.867
131.615

20 cm
128.633
135.100
133.367

25 cm
128.300
133.233
128.267

Figure 1: FTIR spectra of PVB films made by different methods.

To understand the interesting PVB film wettability, we firstly examined the morphologies of selected PVB films (10% concentration) with spin-coating 250 r/s, bar-coating 6μm, and positive and negative electrospinning with distance of 15 cm. As shown in Figure 2(a), the spin-coating PVB film showed a macroscopically relative smooth surface with SWCA 78.8°; the bar-coating film also had a smooth surface with SWCA 83.3° (Figure 2(b)). Both smooth films showed hydrophilicity. Meanwhile, both the positive and negative electrospun PVB films showed porous rough surfaces, as can be found in Figures 2(c) and 2(d), and the SWCA were 130.8° and 135.7°, respectively. Both the porous rough electrospun films showed hydrophobicity. According to these results, it seems that the surface roughness determined the wettability of the films.

(a)

(b)

(c)

(d)

Figure 2: SEM images of the PVB films made by spin-coating 250 r/s (a), bar-coating 6 μm (b), positive electrospinning 15 cm (c), and negative electrospinning 15 cm (d). The upper inset images showed the water droplet onto these films, and the lower inset images showed the electrospun fiber diameter distributions.

For further investigation, we examined the roughness of the selected films, as shown in Figure 3. It is strange that the macroscopical smooth surfaces shown in Figure 2 have higher roughness than the electrospun films. In our opinion, this case may result from the different surface structures of the films that coating films showed relative dense surface structure, while electrospun films had porous surface structure, as can be seen in Figure 2. For the hydrophobilic coating PVB films [seen in Figures 3(a) and 3(b)], bar-coating ones showed higher roughness than the spin-coating ones with r=3.715>2.351, where r is the factor of the surface roughness. According to the Wenzel model [1, 22],

where , the larger the factor of roughness r is, the smaller will get, and the increasing roughness will make the film more hydrophilic. The case in coating PVB films followed the Wenzel model; consequently the bar-coating films with more roughness showed smaller SWCA than spin-coating ones. Meanwhile, for the electrospun films, the porous and micro-nano surface structures made the Wenzel model not work. As suggested in Figures 3(c) and 3(d) and Figures 2(c) and 2(d), the positive electrospun PVB film with more roughness (r=1.106) had smaller SWCA (130.8°) than that of negative electrospinning PVB film (r=1.076, SWCA 135.7°). In this case, the Cassie model, which gives a composite state that liquids are assumed to only contact the solid through the top of the asperities and air pockets are assumed to be trapped underneath the liquid [1, 22], may be considered; the function can be expressed as

where are the area fractions of the solid on the surface. From (2), one can find that the smaller is, the more hydrophobicity will be obtained. Specifically to the electrospun PVB films, the smaller the fiber diameter is, the smaller will be achieved, and then higher hydrophobicity will be shown [5, 7, 10, 11]. From lower inset images in Figure 2, we can obviously find that negative electrospun PVB fibers had smaller diameters and less uniform and consequently exhibited higher SWCA.

(a)

(b)

(c)

(d)

Figure 3: 3D surface roughness of the prepared PVB films under spin-coating 250 r/s (a), bar-coating 6 μm (b), positive electrospinning 15 cm (c), and negative electrospinning 15 cm (d). The inset images showed the 2D surface roughness of these films.

4. Conclusions

In conclusion, we have prepared several kinds of PVB films through spin-coating, bar-coating, and electrospinning. The FTIR spectra suggested that these films have the same chemical structures. Meanwhile, these films showed different wettability that coating films were hydrophilicity and electrospun films were hydrophobicity. SEM images indicated that the different films showed different physical surface structures, which may introduce the different wettability. Further investigation on the surface roughness confirmed that the wettability of coating films obeyed the Wenzel model, while the electrospun films agreed with the Cassie model. These results may help to understand the mechanism of the PVB films and then guide for its practical application.

Data Availability

The data used to support the findings of this study are available from the corresponding author upon request.

Conflicts of Interest

The authors declare that there are no conflicts of interest regarding the publication of this paper.

Acknowledgments

This work was supported by the National Natural Science Foundation of China (51703102, 51373082, and 51673103), the Shandong Provincial Natural Science Foundation, China (ZR2016EMB09 and ZR2017BEM045), and the Qingdao Postdoctoral Applied Research Project.

References

K. Liu, X. Yao, and L. Jiang, “Recent developments in bio-inspired special wettability,” Chemical Society Reviews, vol. 39, no. 8, p. 3240, 2010.

T. L. Sun, L. Feng, X. F. Gao, and L. Jiang, “Bioinspired surfaces with special wettability,” Accounts of Chemical Research, vol. 38, no. 8, pp. 644–652, 2005.

L. Feng, S. Li, Y. Li et al., “Super-hydrophobic surfaces: from natural to artificial,” Advanced Materials, vol. 14, no. 24, pp. 1857–1860, 2002.

J. C. Zhang, C. Pan, Y. F. Zhu et al., “Achieving thermo-mechano-opto-responsive bitemporal colorful luminescence via multiplexing of dual lanthanides in piezoelectric particles and its multidimensional anticounterfeiting,” Advanced Materials, vol. 30, Article ID 1804644, 2018.

M. N. Liu, X. Yan, and M. H. You, “Reversible photochromic nanofibrous membranes with excellent water/windproof and breathable performance,” Journal of Applied Polymer Science, vol. 135, no. 23, Article ID 46342, 2018.

H. Xu, H. Li, and J. Chang, “Controlled drug release from a polymer matrix by patterned electrospun nanofibers with controllable hydrophobicity,” Journal of Materials Chemistry B, vol. 1, no. 33, p. 4182, 2013.

G. S. Liu, X. Yan, F. F. Yan et al., “In situ electrospinning iodine-based fibrous meshes for antibacterial wound dressing,” Nanoscale Research Letters, vol. 13, Article ID 309, 2018.

J. Zhang, S. Li, D. Ju et al., “Flexible inorganic core-shell nanofibers endowed with tunable multicolor up conversion fluorescence for simultaneous monitoring dual drug delivery,” Chemical Engineering Journal, vol. 349, pp. 554–561, 2018.

N. Wang, Y. Si, J. Yu, H. Fong, and B. Ding, “Nano-fiber/net structured electrospun PVA membrane: effects of formic acid as solvent and crosslinking agent on solution properties and membrane morphological structures,” Materials and Corrosion, vol. 120, pp. 135–143, 2017.

X. Yan, M. H. You, T. Lou et al., “Colorful hydrophobic poly(vinyl butyral)/cationic dye fibrous membranes via a colored solution electrospinning process,” Nanoscale Research Letters, vol. 11, no. 540, 2016.

H. Wu, R. Zhang, Y. Sun et al., “Biomimetic nanofiber patterns with controlled wettability,” Soft Matter, vol. 4, no. 12, p. 2429, 2008.

S. S. Liu, C. H. Zhang, J. G. He et al., “Wetting state transition on hydrophilic microscale rough surface,” Acta Physica Sinica, vol. 62, no. 20, Article ID 206201, 2013.

J. Yang, Y. Pu, D. Miao, and X. Ning, “Fabrication of durably superhydrophobic cotton fabrics by atmospheric pressure plasma treatment with a siloxane precursor,” Polymers, vol. 10, Article ID 460, 2018.

J. B. Boreyko and C. H. Chen, “Restoring superhydrophobicity of lotus leaves with vibration-induced dewetting,” Physical Review Letters, vol. 103, no. 17, Article ID 174502, 2009.

T. Young, “An essay on the cohesion of fluids,” Philosophical Transactions of the Royal Society London, vol. 95, pp. 65–87, 1805.

R. N. Wenzel, “Resistance of solid surfaces to wetting by water,” Industrial and Engineering Chemistry, vol. 28, no. 8, pp. 988–994, 1936.

A. B. D. Cassie and S. Baxter, “Wettability of porous surfaces,” Transactions of the Faraday Society, vol. 40, pp. 546–551, 1944.

D. Quéré, “Wetting and roughness,” Annual Review of Materials Research, vol. 38, pp. 71–99, 2008.

H. Ems and S. Ndao, “Microstructure-alone induced transition from hydrophilic to hydrophobic wetting state on silicon,” Applied Surface Science, vol. 339, pp. 137–143, 2015.

M. Khorasani, H. Mirzadeh, and Z. Kermani, “Wettability of porous polydimethylsiloxane surface: morphology study,” Applied Surface Science, vol. 242, no. 3-4, pp. 339–345, 2005.

Y. Zhang, X. Chen, F. Liu et al., “Enhanced coffee-ring effect via substrate roughness in evaporation of colloidal droplets,” Advances in Condensed Matter Physics, vol. 2018, Article ID 9795654, 9 pages, 2018.

K. Lum, D. Chandler, and J. D. Weeks, “Hydrophobicity at small and large length scales,” The Journal of Physical Chemistry B, vol. 103, no. 22, pp. 4570–4577, 1999.

S. Rajamani, T. M. Truskett, and S. Garde, “Hydrophobic hydration from small to large lengthscales: Understanding and manipulating the crossover,” Proceedings of the National Acadamy of Sciences of the United States of America, vol. 102, no. 27, pp. 9475–9480, 2005.

X. B. Li and Y. Liu, “Wetting mechanisms and models on solid surfaces,” Journal of Functional Materials, vol. 38, pp. 3919–3924, 2007 (Chinese).

W. Chen, D. J. David, W. J. MacKnight, and F. E. Karasz, “Miscibility and Phase Behavior in Blends of Poly(vinyl butyral) and Poly(methyl methacrylate),” Macromolecules , vol. 34, no. 12, pp. 4277–4284, 2001.